ELECTROLESS (AUTOCATALYTIC, CHEMICAL) PLATING by Jim Henry Wear-Cafe
Electroless plating refers to the autocatalytic or chemical tal ions plated to a base substrate. The process differs from deposition of the metal is autocatalytic or continuous. The Electroless
of aqueous meplating in that
Components of the electroless bath include an aqueous solution catalyst, reducing agent(s), complexing agent(s), and bath stabilizer(s) specific metal ion concentration, temperature and pH range.
of metal operating
ions, in a
Unlike conventional electroplating, no electrical current is required for deposition. The electroless bath provides a deposit which follows all contours of the substrate cxactly, without building up at the edges and corners. A sharp edge receives the same thickness of deposit as a blind hole. The base substrate being plated must be catalytic in nature. A properly prepared workpiece provsides a catalyzed surface and, once introduced into the electroless solution, a uniform deposition begins. Minute amounts of the electroless metal (i.e., Ni, Cu) itself will catalyze the reaction, so the deposition is autocatalytic after the original surfaces are coated. Electroless deposition then continues, prov,iding that the metal ion and reducing agent are replenished. If air or evolved gas, however. are trapped in a blind hoie or downward facing cavity, this will prevent electroless deposition in these areas. In electroless plating, metal ions are reduced to metal by the action of chemical reducing agents, which are simply electron donors. The metal ions are electron acceptors which react with electron donors. The catalyst is the substance (workpiece or metallic surface) which accelerates the electroless chemical reaction, allowing oxidation of the reducing agent. The metal ion and reducer concentration must be monitored and controlled closely in order to maintain proper ratios and to maintain the overall chemical balance of the plating bath. The electroless plating deposition rate is controlled by temperature, pH and metal ion/reducer concentration, Each of the particular plating reactions has optimum ranges at which the bath should be operated (Table I). Complexing agent(s) act as metal salt ions availa buffer to help control pH and maintain control over the “free” able to the solution, thus allowing solution stability. The stabilizer(s) act as catalytic inhibitors, retarding potential spontaneous decomposition of the electroless bath. Few stabilizers are used in excess of IO PPM, because an electroless bath has a maximum tolerance to a given stabilizer. Excessive use of stabilization material(s) can result in depletion of plating rate, bath life and poor metallurgical deposit properties. Trace impurities and organic contamination (i.e., degreasing solvents, oil residues, mold releases) in the plating bath will affect deposit prop&es and appearance. Foreign inorganic ions (i.e., heavy metals) can have an equal effect. Improper balance and control will cause deposit roughness, porosity, changes in final color, foreign inclusions and poor adhesion. 401
2c-l 9s c 09 -205’t)
Sulfurio sod SOdlUrn
9.0. I I .o
65 “-88 “C (149”.190°F)
45 “-73 “C (113”.165’F)
85 o-95 “C (I 85 “-203 OF)
Cobalt chloride Cobalt sulfate
Palladium chloride Palladium bromide
2-5pm (0.08-0.2 mil)
2.5-IOpm (0.1-0.4 mil)
Gold cyanide Gold chloride Potassium aurate
2-5pm (0.08-0.2 mil)
Sodium hypophosphite Hydrazine DMAB Triethylamine borane
DMAB Sodium hypophosphite Potassium borohydride Potassium cyanoborohydride
Sodium citrate Citric acid Ammonium chloride Succinic acid
Ammonia Methylamine EDTA
Sodium phosphate Potassium citrate Sodium borate Potassium tartrate EDTA
Urea Thioorganic compounds
Thioorganic compounds Organic cyanides Thiourea Thiocyanates
Alkali metal cyanide Alkali hydrogen fluoride Acetylacetone
Table 1. Typical Electroless Plating Bath Components and Operating Parameters (Continued)
Ammonium hydroxide Sodium hydroxide
Ammonium hydroxide Hydrochloric acid
Potassium hydroxide Phosphoric acid Sulfuric acid
Electroless nickel baths may consist of four types: 1. Alkaline, nickel-phosphorus. 2. Acid, nickel-phosphorus. 3. Alkaline, nickel-boron. 4. Acid, nickel-boron. The chemical reducing agent most commonly used is sodium hypophosphite, others include sodium borohydride, n-dimethylamine borane (DMAB), ndiethylamine borane (DEAB) and hydrazine. Alkaline nickel-phosphorus deposits are generally reduced by sodium hypophosphite. These alkaline baths are formulated mostly at low temperatures for plating on plastics. Deposits provide good solderability for the electronics industry, and energy operating costs are reduced due to some solution’s low operating temperatures, however, less corrosion protection, adhesion to steel and difficulty in processing aluminum due to high pH values are drawbacks. A low temperature bath can produce hard as-deposited values of 700 VHN at 2% phosphorus. The phosphorus content can be varied by changing the operating temperature of the bath. One such bath consists of the following components: Nickel sulfate . . . . . . . . . . . . . . . . . . . Sodium hypophosphite . . . . . . . . . . . . . . . Sodium pyrophosphate . . . . . . . . . . . . . . Triethanolamine . . . . . .. . . . . . . . . . . PH................................ Temperature . . . . . . . . . . . . . . . . . . . . . . . .
30 g/L 30 fl 60 ” 100 ml/L 10.0 30t035”C(86t09S°F)
An example of a high-temperature, alkaline, electroless nickel-phosphorus bath is: Nickel sulfate . . . . _. . . . . . . . . . . . . . . . . . Sodiumcitrate . . . . . . . . . . . . . . . . . . . . . . . . . . Ammonium chloride . . . . . . . . . . . . . . . . . . . . . . . . Sodium hypophosphite . . . . . . . . . . . . . . . . . . . . . . . pH . . . . . . . . . . . . . . . . . . . . . .._............... Temperature . . . . . . . . . . . . . . . . . . . . . . . . . .
33 g/L 84 ” 50 ” 17 ” 9.5 85°C (185°F)
Acid nickel-phosphorus deposits normally consist of 88 to 94% nickel and 6 to 12% phosphorus operating at 77 to 93°C (171 to 200°F) with a pH of 4.4-5.2. The re-
by G.P. Ray
This book covers all the thickness measuring methods commonly utilized in the industry today. Each method is covered in its own chapter, with references to ASTM/IS0 or other specifications and articles. to: METAL FINISHING, Three Univenity Plaza, Hackensack, NJ 07601 For faster service, call (201) 487-3700 or FAX your order to (201) 487-3705
All bmk orders musr be prepaid. W, NJ and MA residents add ~pprqmate sales rax. PIeare m&de $5.00 shipping and handling for debmy ofeach bk via UPS to addrerrer in rhe U.S.: $8.00 for each txak for Air Parcel Posr shipmenr CO Canada; and S2O.W for each bxk for Air Parcel Port rhipmenr CDall ether counuier.
ducing agent is commonly sodium hypophosphite. The pH of the solution is the controlling factor affecting the phosphorus content of the deposit. In general, the higher the pH, the lower the phosphorus content, resulting in deposit property changes. Lower phosphorus containing deposits (i.e., 6%) typically have less corrosion resistance than 9% alloys. Also, deposits containing phosphorus in excess of 8.0% are typically nonmagnetic. When the pH drops below 4.0, subsequent nickel deposition virtually stops. As-deposited nickel-phosphorus hardness is 500 to 600 VHN, while maximum values of 950 VHN or slightly more may be realized by post-heat-treatment of the coating at a temperaturg of 400°C (752°F) for one hour. The temperature is a dominant factor in determining the final deposit hardness. Careful consideration should be given to the choice of temperature so as not to affect structural changes of the base substrate. Additionally, low temperatures are used (116”C/24C”F) to relieve any hydrogen embrittlement that may be produced from pretreatment cycles or subsequent electroless nickel deposition. Post-baking of the deposit produces marked structural changes in hardness, wear and abrasion resistance. Depending upon the temperature, bath composition and phosphorus content, this post-treatment cycle will totally change the initial microcrystalline structure, resulting in nickel phosphides to be precipitated creating a very hard matrix. Complete precipitation of nickel phosphides does not occur at temperatures significantly below 400°C (752°F). In general, deposits with 9.0% phosphorus and above tend to produce lower as-deposited hardness values but give slightly higher hardness when postheat-treated. The coating will discolor above 250°C (482°F) in an air atmosphere. Prevention of coating disccloration can be accomplished in a vacuum, inert or reducing atmosphere oven. Physical properties affected by the post-heat-treatment include increas-
COSTS UP TO 50% Per 100 gallons We Supp& ADDPLATE-M
You suppry Sodium
Technology, Inc. I P.O. Surface Box 8585 . Trenton, NJ 08650 I I
Phone (609) 2594099 Fax (609) 2.= !J7-w, M77 I if!%%? . . ..m_
Your Cost $1.30
per metal SHIPPING IDEAL
Sulfate turnover ECONOMY FOR
ing magnetism, adhesion, tensile sirength ductility, electrical resistivity and corrosion
and electrical resistance.
Thickness of the nickel-phosphorus deposit generally ranges from 2.5 to 250 pm (0.1 to 10.0 mils). Deposits less than 2.5 pm and greater than 625 ,um are currently and successfully being preformed. Thickness measurements can be carried out with magnetic devices, micrometers, coulometrics, beta backscatter and X-ray fluorescence.
is an example
of an acid hypophosphite
Nickel sulfate ....... Sodium acetate ...... Sodium hypophosphite Lead acetate ........ pH ............... Temperature ........
28 g/L 17 ‘I 24 I1 0.0015 ” 4.6 82 to88”C (180 to 190°F)
Alkaline nickel-boron solutions utilize the powerful reducing agent, sodium borohydride, to produce a deposit containing 5 to 6% boron and 94 to 95% nickel by weight. These highly alkaline solutions operate at a pH of 12.0 to 14.0 and temperatures of 90 to 95°C (195 to 205°F). These baths tend to be less stable because of their high alkalinity, and bath decomposition may occur if the pH falls below 12.0. As-deposited hardness values of 650 to 750 VHN are typical. After post-heat-treatment at 400°C (752°F) for one hour, values of 1200 VHN can be produced. The melting point of borohydride reduced denosits is 1080°C (1975°F).
is an example
of a sodium
.. .. .. .. .. ..
bath: Nickel chloride Sodium hydroxide Ethylenediamine, Sodium borohydride Thallium nitrate pH ... . Temperature .
... .... 98% _ .. .. .. .. . .
31 g/L 42 “ 52 I’ 1.2 ” 0.022 * 14.0 93 to 95°C (200 to 205 “F)
Acid nickel-boron varies from 0.1 to 4% boron by weight depending on the bath formulation. The boron content of electroless nickel is reduced by either n-dimethylamine borane (DMAB) or n-diethylamine borane (DEAB). Bath parameters include a pH of 4.8 to 7.5 with an operating temperature range of 65 to 77°C (149 to 171 “F). DMAB or DEAB reduced deposits have a very high melting temperature of 1350°C (246O’F). Baths containing less than 1% boron have excellent solderability and good ultrasonic (wire) bonding characteristics. A typical DMAB reduced bath contains: Nickel sulfate Sodium acetate DMAB . .. . Lead acetate pH . .. . . . Temperature
_ . . . . .
.. .. .. . . .. .. . ..
25 g/L 15 ” 4 “ 0.002 n 5.9 26 “C (78 “F)
Electroless copper deposits are generally applied before electroplating on plastics and other non-conductors providing a conductive base for subsequent plating. These include ABS, polystyrene, modified polyphenylene oxide, PVC, Noryl, polyethylene, polysulfone, structural foam, epoxy and ceramics, In such applications, usually a thin deposit (0.127 pm; 0.05 mil) is applied followed by an additional decorative or protective thickness of copper, nickel or gold deposited electrolytically or electrolessly. The electroless copper in such applications provides good life in corrosive atmospheric and/or environmental exposures. Automotive, appliance, hardware parts, circuit boards, through-hole plating, EMI/RFI shielding of electronic devices and ceramics represent major markets for electroless copper. In through-hole plating of circuit boards, the use of electroless copper has eliminated the need for an electrodeposited flash and provides good electrical conductivity in these hard-to-reach areas. In the pretreatment of circuit boards, the most common method involves an acidic aqueous solution of stannous chloride (SNCI,) and palladium chloride (PdCI,) immersion for subsequent deposition of the electroless copper. Many proprietary activators are available in which these solutions can be used separately or together at room temperature. Palladium drag-in to the electroless copper bath can cause solution decomposition instantly. The pH of an electroless copper bath will greatly influence the brightness of the copper deposit. Usually a value above 12.0 is preferred. A dark deposit may indicate low bath alkalinity and contain cuprous oxide. The plating rate is equally influenced by pH. In formaldehyde-reduced baths an optimum value of 12.0 to 13.0 is generally best.
NI NI NI NI NI NI NI
TEC TEC TEC TEC TEC TEC TEC
200 - Nickel Boron ALK EN - Alkaline Nickel Strike 85 - High Phos Electroless 75 - Bright High Speed Mid Phos 9000 - High Speed Bright Electroless 95 pH Self Regulated Mid Phos 2000 Low Cost Electroless Nickel
INDUSTRIAL PARK ROAD WESTFIELD, MA 01085 PHONE (413) 562-7066 FAX (413) 568-6462
Stability of the bath arid pH are critical. A high pH value (14.0) results in poor solution stability and reduces the bath life. Below about 9.5, solution stability is good, however, deposition slows or ceases. The best known reducing agent for electroless copper baths is formaldehyde. The complexing agent serves to complex the copper ion to prevent solution precipitation and has an effect on deposition rates plus quality of the deposit. These conventional baths are stable, have plating rates of 1 to 5 pm or 0.04 to 0.2 mil/hr, and operate in an alkaline solution (pH 10.0 to 13.0). An example of a formaldehyde reduced electroless copper bath is: Copper sulfate . . . . . . . _ . . . . . . . . . . . . 15 g/L Rochellesalt .... . . . ...... . . . 40 ” Formaldehyde (37%) . . . . . . . . . . . . . . . . . 6 ml/L Vanadium oxide . . . . .. . . . . . .. . .OOl g/L pH . . . . . . . . . , . . . . . . . . . . . . . . . . . . . 12.0 Temperature . . . . . . . . . . . . . . . . . . . . . . . 70-75°C (158-167°F) Recent proprietary formulations allow for sodium hypophosphite reduced baths. These high speed (>lO pm/hr. X.4 mil/hr.) or heavy deposition baths generally operate at a lower pH without the use of formaldehyde. High speed baths generally are more expensive and exhibit less stability but have non-harmful formaldehyde vapors given off during subsequent solution make up, heating and deposition. These baths can deposit sufficient low stress copper eliminating the need of an electrolytic flash. Electroless
There is a growing need in the electronic industry for selective plating to conserve plating costs and to allow the electronics engineer freedom for circuit design improve-
Technology beyond the existing state of the art’” Patented Equipment Designs Advanced Techniques . Patented Propriatary Chemistry Simultaneous Plating of Ferrous and Non-Ferrous Metals Worldwide Unexcelled Quality Industrial and M.I.L. Spec. Approved Heavy Deposits to 0.020 In House EN Seminars Superior Corrosion Resistance Introducing Patented [email protected]
PLUS’” CF, Composite l
l l l l
International, Inc. has exclusively specialized in this complex chemical reduction process for the past 24 years supplying a full range of services. We guarantee competitive costing. Specification Quality Assurance, rapid turn-around and consistant deposit metallurgy. In short, [email protected]
‘” is Tomorrow’s Technology...Today!
101 Tenth Street, Rock Island, IL 61201 ‘.O. Box 4177, Rock Island, IL 61204-4177 309) 793-1250 FAX (309) 766-6556
United States, Great Sritan, Ireland, Europe, Asia I T MAKES CENTS T O SPECIFY WEAR-COTE * ” D 1994 Wear-Cole International, Inc.
ment. Many electronic components today are difficult to gold plate by electrolytic means. Thus, electroless gold is one such selective plating currently being used in the fabrication of semiconductor devices, connector tabs, chips and other metalized ceramics. Many commercially available electroless gold baths are produced by immersion plating techniques, however, there are a few true autocatalytic gold processes available with 99.99% purity. Electroless gold can successfully be applied to Kovar, nickel, less nickel, copper, copper alloys, electroless copper and metalized gold can be deposited onto already present thin electrodeposited strength. The following
is an example
of an electroless
Gold chloride hydrochloride trihydrate Sodium potassium tartrate ......... Dimethylamine borane ............ Sodium cyanide .................. pH (adjusted with NaOH) .......... Temperature .................... Electroless
nickel alloys, electroceramics. Electroless gold to give added
. 0.01 moles/L . 0.014 ” . 0.013 ” . 400.0 mg/L . 13.0 60°C (140°F)
Palladium deposits are ductile and ideal for contacts undergoing flexing (i.e., printed circuit board end-connectors and electronic switch contacts). Palladium has also been used as a less expensive replacement for gold providing tarnish resistance and solderability. Using specific bath components, the deposit can be hard and bond to electroless nickel with a bond strength greater than the tensile strength of the palladium plate itself. The electroless nickel preplate can be either from a pyrophosphite or boron reduced bath. The following is an example of an electroless palladium (hypophosphite reduced) bath: Palladium chloride . . . Rochelle salt . . . Ethylenediamine . . .... . . Cool solution to 20 “C (68 “F) and then add sodium hypophosphite . .. . . . . . .. . pH (adjusted with HCl) . . . . .. Temperature . . .. .. . . . . . . . . . . Electroless
10 g/L 19 ” 25.6 ” 4.1 ” 8.5 68-73°C
Thin electroless cobalt deposits have had limited use in the electronics industry magnetic memory discs and storage devices primarily for their magnetic properties. The following
is an example
Cobalt chloride .. . Sodium hypophosphite Sodium citrate . .. . . Ammonium chloride . pH . . . . . . . . . . . . . . . Temperature . .
of an electroless
. . .. .. . .
bath: 30 g/L 20 ” 35 ” 50 ” 9.5 95 “C (203 “F) 413
The uniform dispersion of micron (
molds for rubber and plastic components, fasteners, precision components, drills, gauge blocks, tape recording heads and
Due to the resultant matrix surface topography (when using diamonds or silicon carbide, for example), the final surface roughness must be considered. Special postplate surface finish operations must be employed to regain the required RMS (microinch) finish. In severe abrasion applications involving high pressure foundry molding, it has been noted that the softer electroless nickel matrix wears first, exposing harder composite particles which create poor drawability of the resin/binder from the mold. Polyalloys have been developed to produce deposits having three or four elements with specific coating properties. These include applications where unique chemical and high temperature resistance or electrical, magnetic or non-magnetic properties are requirements. The use of nickel-cobalt-iron-phosphorus polyalloys produce magnetic (for memory) properties. Other polyalloys include nickel-iron-phosphorus, nickel-cobaltnickel-molybdenumphosphorus, nickel-iron-boron, nickel-tungsten-phosphorus, boron, nickel-tungsten-tin-phosphorus, and nickel-copper-phosphorus. The final selection is dependent upon the final application and the economics of achieving the results required. Electroless metal composites and polyalloys have made unique contributions to various engineering applications. Extensive field testing is ongoing to gain experience for proper applications, inclusions and sizes, plus proper electroless bath operating parameters for this new form of electroless plating.